#------------------------------------------------------------------------------
#$Date: 2016-03-23 20:47:22 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179424 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/21/4332147.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the Crystal Eye server at
# http://wwmm.ch.cam.ac.uk/crystaleye/, created by Nick Day at the
# Peter Murray-Rust laboratory.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_4332147
loop_
_publ_author_name
'Birkedal, Henrik'
'Krogh Andersen, Anne Marie'
'Arakcheeva, Alla'
'Chapuis, Gervais'
'Norby, Poul'
'Pattison, Philip'
_publ_section_title
;
 The Room-Temperature Superstructure of ZrP2O7Is Orthorhombic: 
 There Are No Unusual 180° P−O−P Bond Angles
;
_journal_issue                   11
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4346
_journal_page_last               4351
_journal_paper_doi               10.1021/ic0600174
_journal_volume                  45
_journal_year                    2006
_chemical_formula_moiety         'O7 P2 Zr'
_chemical_formula_sum            'O7 P2 Zr'
_chemical_formula_weight         265.16
_chemical_name_common            'Zirconium pyrophosphate'
_chemical_name_systematic
; 
 Zirconium pyrophosphate 
;
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            108
_cell_length_a                   24.7390(2)
_cell_length_b                   24.71841(19)
_cell_length_c                   24.7431(2)
_cell_measurement_temperature    293(2)
_cell_volume                     15130.6(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_radiation_monochromator  silicon
_diffrn_radiation_source         'synchrotron, BM-1 at ESRF'
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1122
_diffrn_reflns_av_sigmaI/netI    0.0376
_diffrn_reflns_limit_h_max       37
_diffrn_reflns_limit_h_min       -37
_diffrn_reflns_limit_k_max       37
_diffrn_reflns_limit_k_min       -37
_diffrn_reflns_limit_l_max       37
_diffrn_reflns_limit_l_min       -37
_diffrn_reflns_number            532466
_diffrn_reflns_theta_full        32.76
_diffrn_reflns_theta_max         32.76
_diffrn_reflns_theta_min         1.65
_exptl_absorpt_coefficient_mu    2.511
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.143
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             13608
_exptl_crystal_size_max          0.02
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.02
_refine_diff_density_max         1.820
_refine_diff_density_min         -2.535
_refine_diff_density_rms         0.235
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.082
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1222
_refine_ls_number_reflns         27901
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.082
_refine_ls_R_factor_all          0.0645
_refine_ls_R_factor_gt           0.0493
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1100P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1522
_refine_ls_wR_factor_ref         0.1619
_reflns_number_gt                22764
_reflns_number_total             27901
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0600174sup1.cif
_cod_data_source_block           all-nomerwght-renam
_cod_original_sg_symbol_H-M      Pbca
_cod_database_code               4332147
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x+1/2, y, -z+1/2'
'-x+1/2, y+1/2, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'-x-1/2, -y, z-1/2'
'x-1/2, -y-1/2, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Zr1 Zr 0.0000 0.5000 0.5000 0.00541(9) Uani 1 2 d S
Zr2 Zr 0.332550(13) 0.497143(13) 0.504037(13) 0.00589(7) Uani 1 1 d .
Zr3 Zr 0.326481(14) 0.167285(12) 0.157576(14) 0.00540(6) Uani 1 1 d .
Zr4 Zr 0.334336(12) 0.177117(14) 0.838964(13) 0.00468(6) Uani 1 1 d .
Zr5 Zr 0.323033(15) 0.497636(12) 0.830673(13) 0.00482(6) Uani 1 1 d .
Zr6 Zr 0.329873(13) 0.832550(12) 0.166986(12) 0.00557(7) Uani 1 1 d .
Zr7 Zr 0.335800(12) 0.664334(12) 0.338937(14) 0.00467(6) Uani 1 1 d .
Zr8 Zr 0.337745(13) 0.159612(14) 0.499704(11) 0.00471(6) Uani 1 1 d .
Zr9 Zr 0.499266(12) 0.496500(12) 0.325957(15) 0.00521(7) Uani 1 1 d .
Zr10 Zr 0.158781(14) 0.331808(13) 0.495136(13) 0.00531(6) Uani 1 1 d .
Zr11 Zr 0.164797(13) 0.499587(12) 0.667854(13) 0.00545(7) Uani 1 1 d .
Zr12 Zr 0.000854(12) 0.165110(12) 0.836988(14) 0.00535(7) Uani 1 1 d .
Zr13 Zr 0.000933(12) 0.165351(12) 0.173155(15) 0.00494(7) Uani 1 1 d .
Zr14 Zr -0.002518(12) 0.159091(15) 0.497818(13) 0.00517(7) Uani 1 1 d .
P1A P 0.13200(3) 0.13298(3) 0.13024(3) 0.00618(14) Uani 1 1 d .
P1B P 0.19750(3) 0.20177(3) 0.20614(3) 0.00663(14) Uani 1 1 d .
O1 O 0.16515(15) 0.18076(13) 0.15561(12) 0.0295(8) Uani 1 1 d .
O1A O 0.07589(11) 0.13608(13) 0.15250(13) 0.0249(7) Uani 1 1 d .
O1B O 0.13310(12) 0.14541(11) 0.07083(10) 0.0179(5) Uani 1 1 d .
O1C O 0.15895(12) 0.08071(11) 0.14457(13) 0.0235(6) Uani 1 1 d .
O1D O 0.18547(12) 0.26168(10) 0.20807(11) 0.0181(5) Uani 1 1 d .
O1E O 0.25616(12) 0.19181(13) 0.19457(13) 0.0248(6) Uani 1 1 d .
O1F O 0.17729(11) 0.17247(11) 0.25596(10) 0.0162(5) Uani 1 1 d .
P2A P 0.13566(3) 0.13331(3) 0.47436(3) 0.00611(14) Uani 1 1 d .
P2B P 0.20867(3) 0.20524(3) 0.53934(3) 0.00628(14) Uani 1 1 d .
O2 O 0.15936(12) 0.16958(13) 0.52103(12) 0.0246(7) Uani 1 1 d .
O2A O 0.15623(13) 0.07726(12) 0.48399(14) 0.0274(7) Uani 1 1 d .
O2B O 0.07576(10) 0.13723(12) 0.48281(12) 0.0209(6) Uani 1 1 d .
O2C O 0.15432(12) 0.15618(11) 0.42130(10) 0.0177(5) Uani 1 1 d .
O2D O 0.21083(10) 0.19718(11) 0.59999(10) 0.0140(5) Uani 1 1 d .
O2E O 0.19521(12) 0.26250(11) 0.52410(12) 0.0213(6) Uani 1 1 d .
O2F O 0.25900(11) 0.18572(12) 0.51176(11) 0.0188(6) Uani 1 1 d .
P3A P 0.13069(3) 0.12599(3) 0.79368(3) 0.00650(14) Uani 1 1 d .
P3B P 0.19747(3) 0.20108(3) 0.86211(3) 0.00548(14) Uani 1 1 d .
O3 O 0.18014(12) 0.15594(12) 0.82070(14) 0.0255(7) Uani 1 1 d .
O3A O 0.12938(12) 0.14383(12) 0.73522(11) 0.0199(6) Uani 1 1 d .
O3B O 0.14568(11) 0.06698(10) 0.79752(12) 0.0175(5) Uani 1 1 d .
O3C O 0.07960(11) 0.13978(11) 0.82310(11) 0.0175(5) Uani 1 1 d .
O3D O 0.25769(10) 0.20302(11) 0.85717(12) 0.0169(5) Uani 1 1 d .
O3E O 0.18017(13) 0.18392(14) 0.91722(12) 0.0282(7) Uani 1 1 d .
O3F O 0.17030(11) 0.25292(10) 0.84501(12) 0.0162(5) Uani 1 1 d .
P4A P 0.13081(3) 0.69660(3) 0.28869(3) 0.00578(14) Uani 1 1 d .
P4B P 0.20028(3) 0.63441(3) 0.36595(3) 0.00565(14) Uani 1 1 d .
O4 O 0.16010(12) 0.64834(11) 0.31813(11) 0.0193(6) Uani 1 1 d .
O4A O 0.13463(11) 0.68316(11) 0.22948(10) 0.0169(5) Uani 1 1 d .
O4B O 0.07301(11) 0.69611(12) 0.30767(12) 0.0201(6) Uani 1 1 d .
O4C O 0.15870(11) 0.74845(10) 0.30247(11) 0.0159(5) Uani 1 1 d .
O4D O 0.20142(11) 0.57334(10) 0.36674(11) 0.0147(5) Uani 1 1 d .
O4E O 0.17810(11) 0.65816(10) 0.41743(10) 0.0159(5) Uani 1 1 d .
O4F O 0.25427(11) 0.65810(11) 0.35099(12) 0.0198(6) Uani 1 1 d .
P5A P 0.12813(3) 0.46227(3) 0.13312(3) 0.00633(14) Uani 1 1 d .
P5B P 0.20291(3) 0.53280(3) 0.19722(3) 0.00604(14) Uani 1 1 d .
O5 O 0.15314(12) 0.49657(13) 0.18095(12) 0.0250(7) Uani 1 1 d .
O5A O 0.15433(11) 0.40728(11) 0.13331(12) 0.0186(6) Uani 1 1 d .
O5B O 0.06897(10) 0.45927(11) 0.14714(11) 0.0136(5) Uani 1 1 d .
O5C O 0.13816(13) 0.49142(11) 0.08097(11) 0.0203(6) Uani 1 1 d .
O5D O 0.20561(11) 0.52838(11) 0.25780(11) 0.0177(5) Uani 1 1 d .
O5E O 0.19191(13) 0.58934(11) 0.17944(13) 0.0260(7) Uani 1 1 d .
O5F O 0.25270(11) 0.50980(12) 0.17057(11) 0.0171(5) Uani 1 1 d .
P6A P 0.13474(3) 0.80077(3) 0.13214(3) 0.00582(14) Uani 1 1 d .
P6B P 0.19963(3) 0.86911(3) 0.20947(3) 0.00614(14) Uani 1 1 d .
O6 O 0.16998(15) 0.82080(12) 0.18148(13) 0.0279(7) Uani 1 1 d .
O6A O 0.15015(12) 0.74172(10) 0.12739(11) 0.0177(5) Uani 1 1 d .
O6B O 0.07628(11) 0.80854(13) 0.14762(13) 0.0255(7) Uani 1 1 d .
O6C O 0.15007(11) 0.83346(10) 0.08277(10) 0.0150(5) Uani 1 1 d .
O6D O 0.19168(12) 0.85906(11) 0.26905(10) 0.0176(5) Uani 1 1 d .
O6E O 0.17381(11) 0.92083(11) 0.19113(13) 0.0200(6) Uani 1 1 d .
O6F O 0.25836(11) 0.86497(12) 0.19390(12) 0.0208(6) Uani 1 1 d .
P7A P 0.12832(3) 0.46193(3) 0.45836(3) 0.00581(14) Uani 1 1 d .
P7B P 0.19745(3) 0.52736(3) 0.53367(3) 0.00654(14) Uani 1 1 d .
O7 O 0.17013(16) 0.47993(13) 0.50212(16) 0.0406(11) Uani 1 1 d .
O7A O 0.15096(14) 0.47633(13) 0.40412(13) 0.0281(7) Uani 1 1 d .
O7B O 0.12370(11) 0.40169(10) 0.46610(11) 0.0161(5) Uani 1 1 d .
O7C O 0.07566(11) 0.49094(11) 0.46827(12) 0.0188(6) Uani 1 1 d .
O7D O 0.25671(11) 0.51522(12) 0.53185(12) 0.0218(6) Uani 1 1 d .
O7E O 0.17438(12) 0.52405(13) 0.58952(11) 0.0244(7) Uani 1 1 d .
O7F O 0.18398(12) 0.57992(10) 0.50649(12) 0.0190(6) Uani 1 1 d .
P8A P 0.13365(3) 0.46811(3) 0.80270(3) 0.00602(14) Uani 1 1 d .
P8B P 0.19667(3) 0.54395(3) 0.87268(3) 0.00626(14) Uani 1 1 d .
O8 O 0.14878(12) 0.51881(11) 0.83861(13) 0.0208(6) Uani 1 1 d .
O8A O 0.07265(10) 0.46789(11) 0.80284(11) 0.0156(5) Uani 1 1 d .
O8B O 0.15657(12) 0.47739(13) 0.74730(11) 0.0206(6) Uani 1 1 d .
O8C O 0.15751(10) 0.41842(10) 0.82863(10) 0.0128(5) Uani 1 1 d .
O8D O 0.18185(11) 0.60330(9) 0.87637(10) 0.0129(5) Uani 1 1 d .
O8E O 0.24875(11) 0.53387(11) 0.84326(11) 0.0170(5) Uani 1 1 d .
O8F O 0.19652(15) 0.51728(12) 0.92737(11) 0.0260(7) Uani 1 1 d .
P9A P 0.13214(3) 0.79393(3) 0.47120(3) 0.00641(14) Uani 1 1 d .
P9B P 0.21170(3) 0.86623(3) 0.52813(3) 0.00671(14) Uani 1 1 d .
O9 O 0.18593(12) 0.82154(13) 0.49050(15) 0.0287(7) Uani 1 1 d .
O9A O 0.13503(12) 0.79436(11) 0.41032(11) 0.0194(6) Uani 1 1 d .
O9B O 0.13424(12) 0.73662(10) 0.49253(12) 0.0201(6) Uani 1 1 d .
O9C O 0.08411(10) 0.82403(11) 0.49269(12) 0.0166(5) Uani 1 1 d .
O9D O 0.26882(10) 0.87193(11) 0.50676(11) 0.0149(5) Uani 1 1 d .
O9E O 0.21108(12) 0.84458(12) 0.58467(11) 0.0219(6) Uani 1 1 d .
O9F O 0.17935(11) 0.91705(11) 0.52206(13) 0.0203(6) Uani 1 1 d .
P10A P 0.46838(3) 0.69844(3) 0.30724(3) 0.00621(14) Uani 1 1 d .
P10B P 0.54319(3) 0.62429(3) 0.36844(3) 0.00650(14) Uani 1 1 d .
O10 O 0.52036(12) 0.67216(12) 0.33324(14) 0.0256(7) Uani 1 1 d .
O10A O 0.47312(11) 0.75747(10) 0.32072(12) 0.0178(5) Uani 1 1 d .
O10B O 0.47074(12) 0.68812(12) 0.24774(11) 0.0208(6) Uani 1 1 d .
O10C O 0.41868(10) 0.67269(11) 0.33172(11) 0.0152(5) Uani 1 1 d .
O10D O 0.51785(11) 0.62620(11) 0.42350(11) 0.0185(5) Uani 1 1 d .
O10E O 0.53092(13) 0.57201(11) 0.34002(11) 0.0203(6) Uani 1 1 d .
O10F O 0.60290(10) 0.63524(11) 0.37138(11) 0.0153(5) Uani 1 1 d .
P11A P 0.45661(3) 0.46476(3) 0.80028(3) 0.00537(14) Uani 1 1 d .
P11B P 0.53254(3) 0.52940(3) 0.86782(3) 0.00576(14) Uani 1 1 d .
O11 O 0.48266(12) 0.49300(12) 0.85151(11) 0.0196(6) Uani 1 1 d .
O11A O 0.48053(11) 0.40881(10) 0.79594(11) 0.0168(5) Uani 1 1 d .
O11B O 0.39720(10) 0.46252(10) 0.81287(11) 0.0142(5) Uani 1 1 d .
O11C O 0.46982(11) 0.49887(10) 0.75154(10) 0.0148(5) Uani 1 1 d .
O11D O 0.53610(11) 0.52211(11) 0.92829(10) 0.0167(5) Uani 1 1 d .
O11E O 0.52003(13) 0.58676(11) 0.85185(13) 0.0242(6) Uani 1 1 d .
O11F O 0.58203(10) 0.50864(11) 0.83901(10) 0.0141(5) Uani 1 1 d .
P12A P 0.47026(3) 0.13132(3) 0.46075(3) 0.00586(14) Uani 1 1 d .
P12B P 0.52982(3) 0.20883(3) 0.53278(3) 0.00670(14) Uani 1 1 d .
O12 O 0.50194(14) 0.18250(11) 0.48184(12) 0.0252(7) Uani 1 1 d .
O12A O 0.41474(11) 0.13302(12) 0.48526(12) 0.0213(6) Uani 1 1 d .
O12B O 0.46976(12) 0.13973(11) 0.40019(10) 0.0167(5) Uani 1 1 d .
O12C O 0.50025(11) 0.08074(10) 0.47673(12) 0.0156(5) Uani 1 1 d .
O12D O 0.50674(11) 0.26527(10) 0.53689(11) 0.0155(5) Uani 1 1 d .
O12E O 0.58901(11) 0.21047(11) 0.51891(13) 0.0219(6) Uani 1 1 d .
O12F O 0.51763(12) 0.17534(10) 0.58189(11) 0.0167(5) Uani 1 1 d .
P13A P 0.46089(3) 0.79556(3) 0.12683(3) 0.00586(14) Uani 1 1 d .
P13B P 0.53350(3) 0.86167(3) 0.20061(3) 0.00606(14) Uani 1 1 d .
O13 O 0.48649(14) 0.83919(14) 0.16456(16) 0.0347(9) Uani 1 1 d .
O13A O 0.40080(10) 0.80304(11) 0.13417(11) 0.0171(5) Uani 1 1 d .
O13B O 0.47889(13) 0.80779(12) 0.06996(12) 0.0239(6) Uani 1 1 d .
O13C O 0.47919(12) 0.74043(11) 0.14346(13) 0.0222(6) Uani 1 1 d .
O13D O 0.51984(14) 0.84447(12) 0.25719(12) 0.0261(7) Uani 1 1 d .
O13E O 0.58634(11) 0.83914(11) 0.18163(12) 0.0194(6) Uani 1 1 d .
O13F O 0.53133(11) 0.92199(10) 0.19296(13) 0.0201(6) Uani 1 1 d .
P14 P 0.46461(3) 0.46978(3) 0.45999(3) 0.00734(15) Uani 1 1 d .
O14 O 0.5139(3) 0.4971(4) 0.4919(3) 0.0389(19) Uani 0.50 1 d P
O14A O 0.47285(14) 0.49377(12) 0.40512(12) 0.0263(7) Uani 1 1 d .
O14B O 0.40824(16) 0.47755(18) 0.47860(19) 0.0558(14) Uani 1 1 d .
O14C O 0.48251(14) 0.41192(12) 0.46237(14) 0.0296(8) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Zr Zr -2.9673 0.5597 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O7C Zr1 O7C 180.00(15) . 5_566
O7C Zr1 O11D 92.13(12) . 6_665
O7C Zr1 O11D 87.87(12) 5_566 6_665
O7C Zr1 O11D 87.87(12) . 2_456
O7C Zr1 O11D 92.13(12) 5_566 2_456
O11D Zr1 O11D 180.0 6_665 2_456
O7C Zr1 O12C 90.09(11) . 3
O7C Zr1 O12C 89.91(11) 5_566 3
O11D Zr1 O12C 90.85(11) 6_665 3
O11D Zr1 O12C 89.15(11) 2_456 3
O7C Zr1 O12C 89.91(11) . 7_566
O7C Zr1 O12C 90.09(11) 5_566 7_566
O11D Zr1 O12C 89.15(11) 6_665 7_566
O11D Zr1 O12C 90.84(11) 2_456 7_566
O12C Zr1 O12C 180.00(14) 3 7_566
O14B Zr2 O7D 178.08(14) . .
O14B Zr2 O9F 88.26(15) . 3_545
O7D Zr2 O9F 90.34(12) . 3_545
O14B Zr2 O5C 89.70(17) . 6_666
O7D Zr2 O5C 88.96(12) . 6_666
O9F Zr2 O5C 88.97(12) 3_545 6_666
O14B Zr2 O8F 89.72(18) . 6_665
O7D Zr2 O8F 91.57(13) . 6_665
O9F Zr2 O8F 89.02(12) 3_545 6_665
O5C Zr2 O8F 177.93(11) 6_666 6_665
O14B Zr2 O2A 91.74(15) . 3
O7D Zr2 O2A 89.70(13) . 3
O9F Zr2 O2A 178.55(13) 3_545 3
O5C Zr2 O2A 92.47(12) 6_666 3
O8F Zr2 O2A 89.53(13) 6_665 3
O10F Zr3 O9E 91.35(11) 4_645 6_665
O10F Zr3 O5E 85.31(12) 4_645 3_545
O9E Zr3 O5E 89.83(13) 6_665 3_545
O10F Zr3 O1E 172.39(12) 4_645 .
O9E Zr3 O1E 92.89(12) 6_665 .
O5E Zr3 O1E 88.39(13) 3_545 .
O10F Zr3 O4A 88.70(11) 4_645 3_545
O9E Zr3 O4A 177.03(12) 6_665 3_545
O5E Zr3 O4A 93.13(12) 3_545 3_545
O1E Zr3 O4A 87.39(12) . 3_545
O10F Zr3 O6A 88.82(11) 4_645 3_545
O9E Zr3 O6A 86.34(12) 6_665 3_545
O5E Zr3 O6A 172.91(12) 3_545 3_545
O1E Zr3 O6A 97.75(12) . 3_545
O4A Zr3 O6A 90.68(11) 3_545 3_545
O9A Zr4 O6D 173.74(11) 6_666 6_666
O9A Zr4 O3D 92.60(12) 6_666 .
O6D Zr4 O3D 91.79(12) 6_666 .
O9A Zr4 O4C 92.27(11) 6_666 6_666
O6D Zr4 O4C 92.63(11) 6_666 6_666
O3D Zr4 O4C 83.95(11) . 6_666
O9A Zr4 O13E 85.87(12) 6_666 5_666
O6D Zr4 O13E 90.31(12) 6_666 5_666
O3D Zr4 O13E 172.93(11) . 5_666
O4C Zr4 O13E 89.21(11) 6_666 5_666
O9A Zr4 O8D 89.40(11) 6_666 3_545
O6D Zr4 O8D 86.13(10) 6_666 3_545
O3D Zr4 O8D 89.90(11) . 3_545
O4C Zr4 O8D 173.69(10) 6_666 3_545
O13E Zr4 O8D 96.98(11) 5_666 3_545
O7A Zr5 O5D 178.13(13) 6_666 6_666
O7A Zr5 O3B 88.49(13) 6_666 3
O5D Zr5 O3B 92.35(11) 6_666 3
O7A Zr5 O4D 88.58(13) 6_666 6_666
O5D Zr5 O4D 90.71(11) 6_666 6_666
O3B Zr5 O4D 174.75(11) 3 6_666
O7A Zr5 O8E 90.54(13) 6_666 .
O5D Zr5 O8E 87.76(12) 6_666 .
O3B Zr5 O8E 91.93(11) 3 .
O4D Zr5 O8E 92.45(11) 6_666 .
O7A Zr5 O11B 92.43(12) 6_666 .
O5D Zr5 O11B 89.30(11) 6_666 .
O3B Zr5 O11B 86.05(11) 3 .
O4D Zr5 O11B 89.73(10) 6_666 .
O8E Zr5 O11B 176.36(11) . .
O3A Zr6 O6F 92.59(12) 6_665 .
O3A Zr6 O1D 85.78(11) 6_665 3
O6F Zr6 O1D 90.75(12) . 3
O3A Zr6 O5A 89.11(11) 6_665 3
O6F Zr6 O5A 86.84(12) . 3
O1D Zr6 O5A 174.25(11) 3 3
O3A Zr6 O13A 90.38(11) 6_665 .
O6F Zr6 O13A 175.47(11) . .
O1D Zr6 O13A 92.88(11) 3 .
O5A Zr6 O13A 89.80(12) 3 .
O3A Zr6 O2D 175.77(11) 6_665 6_665
O6F Zr6 O2D 88.81(11) . 6_665
O1D Zr6 O2D 90.21(11) 3 6_665
O5A Zr6 O2D 94.95(11) 3 6_665
O13A Zr6 O2D 88.46(10) . 6_665
O4F Zr7 O3F 89.53(11) . 6_665
O4F Zr7 O2C 88.02(12) . 3
O3F Zr7 O2C 91.94(11) 6_665 3
O4F Zr7 O8C 91.29(11) . 6_665
O3F Zr7 O8C 177.08(11) 6_665 6_665
O2C Zr7 O8C 90.89(11) 3 6_665
O4F Zr7 O10C 176.30(12) . .
O3F Zr7 O10C 88.84(11) 6_665 .
O2C Zr7 O10C 88.71(11) 3 .
O8C Zr7 O10C 90.50(10) 6_665 .
O4F Zr7 O1F 89.87(12) . 3
O3F Zr7 O1F 87.98(11) 6_665 3
O2C Zr7 O1F 177.88(11) 3 3
O8C Zr7 O1F 89.23(10) 6_665 3
O10C Zr7 O1F 93.40(11) . 3
O9B Zr8 O12A 88.18(12) 3_545 .
O9B Zr8 O7F 175.26(12) 3_545 3_545
O12A Zr8 O7F 87.12(12) . 3_545
O9B Zr8 O4E 89.71(11) 3_545 3_545
O12A Zr8 O4E 89.94(12) . 3_545
O7F Zr8 O4E 90.81(11) 3_545 3_545
O9B Zr8 O2F 92.37(12) 3_545 .
O12A Zr8 O2F 178.08(12) . .
O7F Zr8 O2F 92.35(12) 3_545 .
O4E Zr8 O2F 88.23(11) 3_545 .
O9B Zr8 O6C 87.70(11) 3_545 6_666
O12A Zr8 O6C 93.66(11) . 6_666
O7F Zr8 O6C 92.07(11) 3_545 6_666
O4E Zr8 O6C 175.49(11) 3_545 6_666
O2F Zr8 O6C 88.19(11) . 6_666
O13F Zr9 O10E 176.51(12) 4_645 .
O13F Zr9 O5B 88.94(11) 4_645 2
O10E Zr9 O5B 91.84(12) . 2
O13F Zr9 O8A 90.08(11) 4_645 6_665
O10E Zr9 O8A 89.32(12) . 6_665
O5B Zr9 O8A 176.78(11) 2 6_665
O13F Zr9 O14A 94.04(13) 4_645 .
O10E Zr9 O14A 89.40(12) . .
O5B Zr9 O14A 86.78(12) 2 .
O8A Zr9 O14A 90.23(12) 6_665 .
O13F Zr9 O11C 88.54(11) 4_645 5_666
O10E Zr9 O11C 88.05(11) . 5_666
O5B Zr9 O11C 90.85(11) 2 5_666
O8A Zr9 O11C 92.19(11) 6_665 5_666
O14A Zr9 O11C 176.46(14) . 5_666
O3E Zr10 O12E 87.77(13) 8_565 7_566
O3E Zr10 O1B 174.11(13) 8_565 8_566
O12E Zr10 O1B 91.94(12) 7_566 8_566
O3E Zr10 O7B 86.53(13) 8_565 .
O12E Zr10 O7B 90.78(11) 7_566 .
O1B Zr10 O7B 87.58(11) 8_566 .
O3E Zr10 O2E 93.25(13) 8_565 .
O12E Zr10 O2E 90.19(12) 7_566 .
O1B Zr10 O2E 92.63(12) 8_566 .
O7B Zr10 O2E 178.99(11) . .
O3E Zr10 O9D 89.89(12) 8_565 3_545
O12E Zr10 O9D 177.18(12) 7_566 3_545
O1B Zr10 O9D 90.55(11) 8_566 3_545
O7B Zr10 O9D 90.65(10) . 3_545
O2E Zr10 O9D 88.37(11) . 3_545
O7E Zr11 O8B 178.03(13) . .
O7E Zr11 O5F 87.09(11) . 6_666
O8B Zr11 O5F 92.12(11) . 6_666
O7E Zr11 O6E 88.29(13) . 8_576
O8B Zr11 O6E 89.90(13) . 8_576
O5F Zr11 O6E 89.50(11) 6_666 8_576
O7E Zr11 O11F 90.29(11) . 2_456
O8B Zr11 O11F 90.53(11) . 2_456
O5F Zr11 O11F 177.16(11) 6_666 2_456
O6E Zr11 O11F 91.53(11) 8_576 2_456
O7E Zr11 O1C 91.60(13) . 8_566
O8B Zr11 O1C 90.19(13) . 8_566
O5F Zr11 O1C 88.29(12) 6_666 8_566
O6E Zr11 O1C 177.79(12) 8_576 8_566
O11F Zr11 O1C 90.67(11) 2_456 8_566
O11E Zr12 O6B 91.85(13) 3_545 5_566
O11E Zr12 O13D 90.04(13) 3_545 6_666
O6B Zr12 O13D 89.04(14) 5_566 6_666
O11E Zr12 O10A 176.30(12) 3_545 6_666
O6B Zr12 O10A 91.84(12) 5_566 6_666
O13D Zr12 O10A 89.84(12) 6_666 6_666
O11E Zr12 O12F 89.54(12) 3_545 2_456
O6B Zr12 O12F 88.14(13) 5_566 2_456
O13D Zr12 O12F 177.13(13) 6_666 2_456
O10A Zr12 O12F 90.76(11) 6_666 2_456
O11E Zr12 O3C 88.92(12) 3_545 .
O6B Zr12 O3C 178.46(13) 5_566 .
O13D Zr12 O3C 92.29(12) 6_666 .
O10A Zr12 O3C 87.39(11) 6_666 .
O12F Zr12 O3C 90.53(11) 2_456 .
O4B Zr13 O11A 91.48(12) 4_545 7_566
O4B Zr13 O10B 89.71(12) 4_545 3_545
O11A Zr13 O10B 89.65(11) 7_566 3_545
O4B Zr13 O1A 178.46(12) 4_545 .
O11A Zr13 O1A 90.01(12) 7_566 .
O10B Zr13 O1A 90.69(13) 3_545 .
O4B Zr13 O13C 87.77(12) 4_545 3_545
O11A Zr13 O13C 178.90(13) 7_566 3_545
O10B Zr13 O13C 89.55(12) 3_545 3_545
O1A Zr13 O13C 90.75(12) . 3_545
O4B Zr13 O12B 89.07(12) 4_545 2_455
O11A Zr13 O12B 87.80(10) 7_566 2_455
O10B Zr13 O12B 177.15(12) 3_545 2_455
O1A Zr13 O12B 90.60(13) . 2_455
O13C Zr13 O12B 92.98(11) 3_545 2_455
O2B Zr14 O10D 84.68(12) . 3_545
O2B Zr14 O14C 91.85(14) . 7_566
O10D Zr14 O14C 93.33(13) 3_545 7_566
O2B Zr14 O13B 89.64(12) . 6_666
O10D Zr14 O13B 174.06(12) 3_545 6_666
O14C Zr14 O13B 88.57(13) 7_566 6_666
O2B Zr14 O12D 93.36(12) . 7_566
O10D Zr14 O12D 90.38(11) 3_545 7_566
O14C Zr14 O12D 173.87(14) 7_566 7_566
O13B Zr14 O12D 88.22(12) 6_666 7_566
O2B Zr14 O9C 174.46(12) . 5_566
O10D Zr14 O9C 90.07(11) 3_545 5_566
O14C Zr14 O9C 86.66(13) 7_566 5_566
O13B Zr14 O9C 95.66(12) 6_666 5_566
O12D Zr14 O9C 88.46(11) 7_566 5_566
O1A P1A O1C 111.75(17) . .
O1A P1A O1B 111.51(17) . .
O1C P1A O1B 113.61(17) . .
O1A P1A O1 107.4(2) . .
O1C P1A O1 108.80(19) . .
O1B P1A O1 103.19(16) . .
O1E P1B O1D 110.95(17) . .
O1E P1B O1F 113.34(17) . .
O1D P1B O1F 112.21(16) . .
O1E P1B O1 106.7(2) . .
O1D P1B O1 104.39(17) . .
O1F P1B O1 108.72(17) . .
P1A O1 P1B 146.4(2) . .
P1A O1A Zr13 161.3(2) . .
P1A O1B Zr10 162.36(19) . 8_565
P1A O1C Zr11 157.5(2) . 8_565
P1B O1D Zr6 148.62(18) . 3_545
P1B O1E Zr3 162.1(2) . .
P1B O1F Zr7 153.82(18) . 3_545
O2A P2A O2B 111.96(18) . .
O2A P2A O2C 112.54(17) . .
O2B P2A O2C 113.66(17) . .
O2A P2A O2 106.5(2) . .
O2B P2A O2 103.23(17) . .
O2C P2A O2 108.20(16) . .
O2F P2B O2E 111.89(17) . .
O2F P2B O2D 112.28(16) . .
O2E P2B O2D 112.36(16) . .
O2F P2B O2 109.44(17) . .
O2E P2B O2 106.50(18) . .
O2D P2B O2 103.84(15) . .
P2B O2 P2A 145.0(2) . .
P2A O2A Zr2 167.2(2) . 3_545
P2A O2B Zr14 168.0(2) . .
P2A O2C Zr7 159.53(18) . 3_545
P2B O2D Zr6 145.21(16) . 6_666
P2B O2E Zr10 165.0(2) . .
P2B O2F Zr8 161.01(19) . .
O3C P3A O3B 113.39(16) . .
O3C P3A O3A 112.36(16) . .
O3B P3A O3A 110.34(16) . .
O3C P3A O3 109.96(17) . .
O3B P3A O3 103.67(16) . .
O3A P3A O3 106.55(18) . .
O3E P3B O3D 111.71(18) . .
O3E P3B O3F 111.75(17) . .
O3D P3B O3F 113.19(16) . .
O3E P3B O3 108.40(19) . .
O3D P3B O3 103.94(16) . .
O3F P3B O3 107.35(17) . .
P3B O3 P3A 145.0(2) . .
P3A O3A Zr6 149.28(19) . 6_666
P3A O3B Zr5 157.81(19) . 3_545
P3A O3C Zr12 160.29(18) . .
P3B O3D Zr4 158.23(18) . .
P3B O3E Zr10 174.1(2) . 8_566
P3B O3F Zr7 153.98(18) . 6_666
O4C P4A O4B 111.97(16) . .
O4C P4A O4A 112.46(16) . .
O4B P4A O4A 111.20(16) . .
O4C P4A O4 109.37(15) . .
O4B P4A O4 106.68(17) . .
O4A P4A O4 104.73(16) . .
O4F P4B O4E 112.32(16) . .
O4F P4B O4D 112.07(16) . .
O4E P4B O4D 112.68(15) . .
O4F P4B O4 106.79(17) . .
O4E P4B O4 108.58(16) . .
O4D P4B O4 103.81(15) . .
P4A O4 P4B 143.08(19) . .
P4A O4A Zr3 155.75(18) . 3
P4A O4B Zr13 158.24(19) . 4
P4A O4C Zr4 154.92(18) . 6_665
P4B O4D Zr5 147.22(16) . 6_665
P4B O4E Zr8 154.96(18) . 3
P4B O4F Zr7 160.19(19) . .
O5C P5A O5B 112.52(16) . .
O5C P5A O5A 111.42(16) . .
O5B P5A O5A 111.90(15) . .
O5C P5A O5 108.77(18) . .
O5B P5A O5 103.56(15) . .
O5A P5A O5 108.24(18) . .
O5E P5B O5D 111.75(18) . .
O5E P5B O5F 111.93(18) . .
O5D P5B O5F 111.83(16) . .
O5E P5B O5 108.36(19) . .
O5D P5B O5 104.37(16) . .
O5F P5B O5 108.20(16) . .
P5B O5 P5A 143.3(2) . .
P5A O5A Zr6 152.96(18) . 3_545
P5A O5B Zr9 149.75(17) . 2_455
P5A O5C Zr2 157.16(18) . 6_665
P5B O5D Zr5 152.57(18) . 6_665
P5B O5E Zr3 177.1(2) . 3
P5B O5F Zr11 150.20(18) . 6_665
O6B P6A O6C 112.18(16) . .
O6B P6A O6A 112.59(17) . .
O6C P6A O6A 112.91(15) . .
O6B P6A O6 107.0(2) . .
O6C P6A O6 108.57(16) . .
O6A P6A O6 102.89(17) . .
O6E P6B O6F 113.05(16) . .
O6E P6B O6D 112.38(17) . .
O6F P6B O6D 111.38(17) . .
O6E P6B O6 108.50(17) . .
O6F P6B O6 106.70(19) . .
O6D P6B O6 104.23(17) . .
P6B O6 P6A 147.2(2) . .
P6A O6A Zr3 154.23(18) . 3
P6A O6B Zr12 168.3(2) . 5_566
P6A O6C Zr8 151.20(17) . 6_665
P6B O6D Zr4 159.62(18) . 6_665
P6B O6E Zr11 160.74(19) . 8_575
P6B O6F Zr6 160.1(2) . .
O7A P7A O7B 112.18(17) . .
O7A P7A O7C 110.87(17) . .
O7B P7A O7C 112.60(16) . .
O7A P7A O7 107.8(2) . .
O7B P7A O7 104.11(17) . .
O7C P7A O7 108.9(2) . .
O7D P7B O7E 112.95(17) . .
O7D P7B O7F 112.19(17) . .
O7E P7B O7F 112.11(17) . .
O7D P7B O7 105.0(2) . .
O7E P7B O7 104.8(2) . .
O7F P7B O7 109.25(18) . .
P7A O7 P7B 147.8(2) . .
P7A O7A Zr5 174.4(2) . 6_665
P7A O7B Zr10 147.22(17) . .
P7A O7C Zr1 155.10(18) . .
P7B O7D Zr2 162.0(2) . .
P7B O7E Zr11 159.31(19) . .
P7B O7F Zr8 158.05(19) . 3
O8B P8A O8C 111.45(16) . .
O8B P8A O8A 112.36(16) . .
O8C P8A O8A 112.82(15) . .
O8B P8A O8 107.62(18) . .
O8C P8A O8 108.31(16) . .
O8A P8A O8 103.77(15) . .
O8E P8B O8F 111.45(17) . .
O8E P8B O8D 113.43(15) . .
O8F P8B O8D 111.67(15) . .
O8E P8B O8 108.63(17) . .
O8F P8B O8 107.78(19) . .
O8D P8B O8 103.37(15) . .
P8A O8 P8B 142.0(2) . .
P8A O8A Zr9 149.36(17) . 6_666
P8A O8B Zr11 162.48(19) . .
P8A O8C Zr7 152.93(17) . 6_666
P8B O8D Zr4 150.15(16) . 3
P8B O8E Zr5 155.22(18) . .
P8B O8F Zr2 154.8(2) . 6_666
O9C P9A O9A 112.85(17) . .
O9C P9A O9B 111.60(16) . .
O9A P9A O9B 110.71(16) . .
O9C P9A O9 110.37(16) . .
O9A P9A O9 105.10(18) . .
O9B P9A O9 105.78(18) . .
O9F P9B O9E 112.82(17) . .
O9F P9B O9D 112.68(15) . .
O9E P9B O9D 111.64(16) . .
O9F P9B O9 108.18(18) . .
O9E P9B O9 107.26(19) . .
O9D P9B O9 103.63(16) . .
P9A O9 P9B 145.7(2) . .
P9A O9A Zr4 151.85(19) . 6_665
P9A O9B Zr8 156.75(19) . 3
P9A O9C Zr14 155.64(19) . 5_566
P9B O9D Zr10 144.28(16) . 3
P9B O9E Zr3 151.35(19) . 6_666
P9B O9F Zr2 155.33(18) . 3
O10B P10A O10A 112.42(17) . .
O10B P10A O10C 110.76(16) . .
O10A P10A O10C 112.57(16) . .
O10B P10A O10 107.42(19) . .
O10A P10A O10 104.24(17) . .
O10C P10A O10 109.03(16) . .
O10D P10B O10E 111.57(16) . .
O10D P10B O10F 111.15(16) . .
O10E P10B O10F 112.09(17) . .
O10D P10B O10 109.20(18) . .
O10E P10B O10 108.38(18) . .
O10F P10B O10 104.12(15) . .
P10B O10 P10A 145.8(2) . .
P10A O10A Zr12 166.22(19) . 6_665
P10A O10B Zr13 160.9(2) . 3
P10A O10C Zr7 152.02(18) . .
P10B O10D Zr14 154.96(18) . 3
P10B O10E Zr9 159.75(18) . .
P10B O10F Zr3 153.00(17) . 4_655
O11B P11A O11C 113.49(16) . .
O11B P11A O11A 111.37(15) . .
O11C P11A O11A 111.77(15) . .
O11B P11A O11 104.37(16) . .
O11C P11A O11 107.79(15) . .
O11A P11A O11 107.54(17) . .
O11E P11B O11F 111.33(17) . .
O11E P11B O11D 112.64(17) . .
O11F P11B O11D 112.39(16) . .
O11E P11B O11 108.00(18) . .
O11F P11B O11 108.66(16) . .
O11D P11B O11 103.35(15) . .
P11B O11 P11A 140.7(2) . .
P11A O11A Zr13 152.92(18) . 7_666
P11A O11B Zr5 153.14(17) . .
P11A O11C Zr9 148.56(16) . 5_666
P11B O11D Zr1 149.31(18) . 2_556
P11B O11E Zr12 174.5(2) . 3
P11B O11F Zr11 151.73(17) . 2_556
O12A P12A O12C 111.56(16) . .
O12A P12A O12B 112.87(17) . .
O12C P12A O12B 112.21(16) . .
O12A P12A O12 107.35(18) . .
O12C P12A O12 109.52(16) . .
O12B P12A O12 102.81(16) . .
O12F P12B O12E 113.29(17) . .
O12F P12B O12D 112.26(15) . .
O12E P12B O12D 110.99(16) . .
O12F P12B O12 109.36(16) . .
O12E P12B O12 104.74(19) . .
O12D P12B O12 105.63(17) . .
P12A O12 P12B 144.4(2) . .
P12A O12A Zr8 158.54(19) . .
P12A O12B Zr13 155.08(18) . 2
P12A O12C Zr1 150.30(17) . 3_545
P12B O12D Zr14 147.98(17) . 7_666
P12B O12E Zr10 147.71(18) . 7_666
P12B O12F Zr12 153.48(17) . 2_556
O13C P13A O13B 110.53(17) . .
O13C P13A O13A 112.16(17) . .
O13B P13A O13A 112.27(17) . .
O13C P13A O13 110.0(2) . .
O13B P13A O13 107.5(2) . .
O13A P13A O13 104.08(17) . .
O13E P13B O13D 112.56(18) . .
O13E P13B O13F 111.15(16) . .
O13D P13B O13F 112.96(17) . .
O13E P13B O13 109.73(18) . .
O13D P13B O13 105.3(2) . .
O13F P13B O13 104.68(18) . .
P13A O13 P13B 152.4(3) . .
P13A O13A Zr6 157.97(18) . .
P13A O13B Zr14 168.0(2) . 6_665
P13A O13C Zr13 174.0(2) . 3
P13B O13D Zr12 170.1(2) . 6_665
P13B O13E Zr4 168.25(19) . 5_666
P13B O13F Zr9 159.17(19) . 4_655
O14B P14 O14A 111.1(2) . .
O14B P14 O14C 112.9(2) . .
O14A P14 O14C 111.95(17) . .
O14B P14 O14 90.9(3) . 5_666
O14A P14 O14 116.4(4) . 5_666
O14C P14 O14 112.0(4) . 5_666
O14B P14 O14 120.6(3) . .
O14A P14 O14 100.1(4) . .
O14C P14 O14 99.1(4) . .
P14 O14 P14 150.3(5) 5_666 .
P14 O14A Zr9 156.46(19) . .
P14 O14B Zr2 173.7(3) . .
P14 O14C Zr14 153.0(2) . 7_666
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Zr1 O7C 2.042(3) .
Zr1 O7C 2.042(3) 5_566
Zr1 O11D 2.060(3) 6_665
Zr1 O11D 2.060(3) 2_456
Zr1 O12C 2.077(2) 3
Zr1 O12C 2.077(2) 7_566
Zr2 O14B 2.034(3) .
Zr2 O7D 2.048(3) .
Zr2 O9F 2.051(3) 3_545
Zr2 O5C 2.056(3) 6_666
Zr2 O8F 2.060(3) 6_665
Zr2 O2A 2.060(3) 3
Zr3 O10F 2.048(2) 4_645
Zr3 O9E 2.050(3) 6_665
Zr3 O5E 2.052(3) 3_545
Zr3 O1E 2.057(3) .
Zr3 O4A 2.060(3) 3_545
Zr3 O6A 2.068(2) 3_545
Zr4 O9A 2.046(3) 6_666
Zr4 O6D 2.051(3) 6_666
Zr4 O3D 2.051(3) .
Zr4 O4C 2.057(2) 6_666
Zr4 O13E 2.067(3) 5_666
Zr4 O8D 2.085(2) 3_545
Zr5 O7A 2.032(3) 6_666
Zr5 O5D 2.041(3) 6_666
Zr5 O3B 2.052(3) 3
Zr5 O4D 2.059(2) 6_666
Zr5 O8E 2.068(3) .
Zr5 O11B 2.077(2) .
Zr6 O3A 2.051(3) 6_665
Zr6 O6F 2.053(3) .
Zr6 O1D 2.061(3) 3
Zr6 O5A 2.064(3) 3
Zr6 O13A 2.066(2) .
Zr6 O2D 2.074(3) 6_665
Zr7 O4F 2.045(3) .
Zr7 O3F 2.056(2) 6_665
Zr7 O2C 2.062(3) 3
Zr7 O8C 2.068(2) 6_665
Zr7 O10C 2.069(3) .
Zr7 O1F 2.088(3) 3
Zr8 O9B 2.034(3) 3_545
Zr8 O12A 2.046(3) .
Zr8 O7F 2.049(3) 3_545
Zr8 O4E 2.073(3) 3_545
Zr8 O2F 2.074(3) .
Zr8 O6C 2.084(3) 6_666
Zr9 O13F 2.046(3) 4_645
Zr9 O10E 2.054(3) .
Zr9 O5B 2.065(2) 2
Zr9 O8A 2.066(3) 6_665
Zr9 O14A 2.066(3) .
Zr9 O11C 2.067(3) 5_666
Zr10 O3E 2.037(3) 8_565
Zr10 O12E 2.047(3) 7_566
Zr10 O1B 2.056(3) 8_566
Zr10 O7B 2.062(2) .
Zr10 O2E 2.064(3) .
Zr10 O9D 2.067(3) 3_545
Zr11 O7E 2.044(3) .
Zr11 O8B 2.051(3) .
Zr11 O5F 2.055(3) 6_666
Zr11 O6E 2.062(3) 8_576
Zr11 O11F 2.067(3) 2_456
Zr11 O1C 2.072(3) 8_566
Zr12 O11E 2.038(3) 3_545
Zr12 O6B 2.052(3) 5_566
Zr12 O13D 2.053(3) 6_666
Zr12 O10A 2.059(3) 6_666
Zr12 O12F 2.065(3) 2_456
Zr12 O3C 2.075(3) .
Zr13 O4B 2.037(3) 4_545
Zr13 O11A 2.049(2) 7_566
Zr13 O10B 2.053(3) 3_545
Zr13 O1A 2.055(3) .
Zr13 O13C 2.055(3) 3_545
Zr13 O12B 2.071(3) 2_455
Zr14 O2B 2.044(3) .
Zr14 O10D 2.046(3) 3_545
Zr14 O14C 2.047(3) 7_566
Zr14 O13B 2.049(3) 6_666
Zr14 O12D 2.070(3) 7_566
Zr14 O9C 2.074(3) 5_566
P1A O1A 1.495(3) .
P1A O1C 1.496(3) .
P1A O1B 1.502(3) .
P1A O1 1.569(3) .
P1B O1E 1.499(3) .
P1B O1D 1.511(3) .
P1B O1F 1.515(3) .
P1B O1 1.573(3) .
O1B Zr10 2.056(3) 8_565
O1C Zr11 2.072(3) 8_565
O1D Zr6 2.061(3) 3_545
O1F Zr7 2.088(3) 3_545
P2A O2A 1.495(3) .
P2A O2B 1.500(3) .
P2A O2C 1.502(3) .
P2A O2 1.575(3) .
P2B O2F 1.500(3) .
P2B O2E 1.502(3) .
P2B O2D 1.515(3) .
P2B O2 1.572(3) .
O2A Zr2 2.060(3) 3_545
O2C Zr7 2.062(3) 3_545
O2D Zr6 2.074(3) 6_666
P3A O3C 1.498(3) .
P3A O3B 1.508(3) .
P3A O3A 1.512(3) .
P3A O3 1.579(3) .
P3B O3E 1.491(3) .
P3B O3D 1.495(3) .
P3B O3F 1.508(3) .
P3B O3 1.574(3) .
O3A Zr6 2.051(3) 6_666
O3B Zr5 2.052(3) 3_545
O3E Zr10 2.037(3) 8_566
O3F Zr7 2.056(2) 6_666
P4A O4C 1.495(3) .
P4A O4B 1.505(3) .
P4A O4A 1.505(3) .
P4A O4 1.574(3) .
P4B O4F 1.505(3) .
P4B O4E 1.506(3) .
P4B O4D 1.510(3) .
P4B O4 1.583(3) .
O4A Zr3 2.060(3) 3
O4B Zr13 2.037(3) 4
O4C Zr4 2.057(2) 6_665
O4D Zr5 2.059(2) 6_665
O4E Zr8 2.073(3) 3
P5A O5C 1.499(3) .
P5A O5B 1.506(3) .
P5A O5A 1.506(3) .
P5A O5 1.582(3) .
P5B O5E 1.490(3) .
P5B O5D 1.504(3) .
P5B O5F 1.509(3) .
P5B O5 1.575(3) .
O5A Zr6 2.064(3) 3_545
O5B Zr9 2.065(2) 2_455
O5C Zr2 2.056(3) 6_665
O5D Zr5 2.041(3) 6_665
O5E Zr3 2.052(3) 3
O5F Zr11 2.055(3) 6_665
P6A O6B 1.508(3) .
P6A O6C 1.513(3) .
P6A O6A 1.513(3) .
P6A O6 1.580(3) .
P6B O6E 1.499(3) .
P6B O6F 1.507(3) .
P6B O6D 1.508(3) .
P6B O6 1.563(3) .
O6A Zr3 2.068(2) 3
O6B Zr12 2.052(3) 5_566
O6C Zr8 2.084(3) 6_665
O6D Zr4 2.051(3) 6_665
O6E Zr11 2.062(3) 8_575
P7A O7A 1.497(3) .
P7A O7B 1.506(3) .
P7A O7C 1.507(3) .
P7A O7 1.562(3) .
P7B O7D 1.497(3) .
P7B O7E 1.497(3) .
P7B O7F 1.500(3) .
P7B O7 1.562(3) .
O7A Zr5 2.032(3) 6_665
O7F Zr8 2.049(3) 3
P8A O8B 1.501(3) .
P8A O8C 1.506(3) .
P8A O8A 1.509(3) .
P8A O8 1.581(3) .
P8B O8E 1.501(3) .
P8B O8F 1.505(3) .
P8B O8D 1.515(2) .
P8B O8 1.581(3) .
O8A Zr9 2.066(3) 6_666
O8C Zr7 2.068(2) 6_666
O8D Zr4 2.085(2) 3
O8F Zr2 2.060(3) 6_666
P9A O9C 1.500(3) .
P9A O9A 1.508(3) .
P9A O9B 1.513(3) .
P9A O9 1.570(3) .
P9B O9F 1.497(3) .
P9B O9E 1.498(3) .
P9B O9D 1.515(3) .
P9B O9 1.579(3) .
O9A Zr4 2.046(3) 6_665
O9B Zr8 2.034(3) 3
O9C Zr14 2.074(3) 5_566
O9D Zr10 2.067(3) 3
O9E Zr3 2.050(3) 6_666
O9F Zr2 2.051(3) 3
P10A O10B 1.495(3) .
P10A O10A 1.501(3) .
P10A O10C 1.511(3) .
P10A O10 1.578(3) .
P10B O10D 1.500(3) .
P10B O10E 1.502(3) .
P10B O10F 1.504(3) .
P10B O10 1.574(3) .
O10A Zr12 2.059(2) 6_665
O10B Zr13 2.053(3) 3
O10D Zr14 2.046(3) 3
O10F Zr3 2.048(2) 4_655
P11A O11B 1.503(3) .
P11A O11C 1.507(3) .
P11A O11A 1.508(3) .
P11A O11 1.584(3) .
P11B O11E 1.504(3) .
P11B O11F 1.507(3) .
P11B O11D 1.510(3) .
P11B O11 1.580(3) .
O11A Zr13 2.049(2) 7_666
O11C Zr9 2.067(3) 5_666
O11D Zr1 2.060(3) 2_556
O11E Zr12 2.038(3) 3
O11F Zr11 2.067(3) 2_556
P12A O12A 1.502(3) .
P12A O12C 1.507(3) .
P12A O12B 1.513(3) .
P12A O12 1.577(3) .
P12B O12F 1.501(3) .
P12B O12E 1.504(3) .
P12B O12D 1.511(3) .
P12B O12 1.577(3) .
O12B Zr13 2.071(3) 2
O12C Zr1 2.077(2) 3_545
O12D Zr14 2.070(2) 7_666
O12E Zr10 2.048(3) 7_666
O12F Zr12 2.065(3) 2_556
P13A O13C 1.494(3) .
P13A O13B 1.507(3) .
P13A O13A 1.509(3) .
P13A O13 1.560(3) .
P13B O13E 1.496(3) .
P13B O13D 1.502(3) .
P13B O13F 1.504(3) .
P13B O13 1.568(3) .
O13B Zr14 2.049(3) 6_665
O13C Zr13 2.056(3) 3
O13D Zr12 2.054(3) 6_665
O13E Zr4 2.067(3) 5_666
O13F Zr9 2.046(3) 4_655
P14 O14B 1.481(3) .
P14 O14A 1.496(3) .
P14 O14C 1.498(3) .
P14 O14 1.540(7) 5_666
P14 O14 1.602(7) .
O14 O14 0.808(13) 5_666
O14 P14 1.540(7) 5_666
O14C Zr14 2.047(3) 7_666
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_4
O1A P1A O1 P1B 80.6(5) .
O1B P1A O1 P1B -161.5(5) .
O1C P1A O1 P1B -40.6(5) .
O1D P1B O1 P1A -145.2(5) .
O1E P1B O1 P1A 97.3(5) .
O1F P1B O1 P1A -25.3(5) .
O2A P2A O2 P2B 87.6(4) .
O2B P2A O2 P2B -154.3(4) .
O2C P2A O2 P2B -33.6(5) .
O2D P2B O2 P2A -147.4(4) .
O2E P2B O2 P2A 93.9(4) .
O2F P2B O2 P2A -27.3(5) .
O3A P3A O3 P3B 110.0(4) .
O3B P3A O3 P3B -133.5(4) .
O3C P3A O3 P3B -12.0(5) .
O3D P3B O3 P3A -175.7(4) .
O3E P3B O3 P3A 65.4(5) .
O3F P3B O3 P3A -55.5(5) .
O4A P4A O4 P4B 138.8(3) .
O4B P4A O4 P4B -103.3(4) .
O4C P4A O4 P4B 18.0(4) .
O4D P4B O4 P4A 175.1(3) .
O4E P4B O4 P4A 55.0(4) .
O4F P4B O4 P4A -66.3(4) .
O5A P5A O5 P5B 82.4(4) .
O5B P5A O5 P5B -158.7(4) .
O5C P5A O5 P5B -38.8(4) .
O5D P5B O5 P5A -155.1(4) .
O5E P5B O5 P5A 85.7(4) .
O5F P5B O5 P5A -35.8(4) .
O6A P6A O6 P6B 151.8(5) .
O6B P6A O6 P6B -89.3(5) .
O6C P6A O6 P6B 32.0(5) .
O6D P6B O6 P6A 144.1(5) .
O6E P6B O6 P6A 24.2(5) .
O6F P6B O6 P6A -97.9(5) .
O7A P7A O7 P7B 72.6(6) .
O7B P7A O7 P7B -168.0(6) .
O7C P7A O7 P7B -47.7(7) .
O7D P7B O7 P7A -133.2(6) .
O7E P7B O7 P7A 107.6(6) .
O7F P7B O7 P7A -12.7(7) .
O8A P8A O8 P8B 160.0(3) .
O8B P8A O8 P8B -80.7(4) .
O8C P8A O8 P8B 39.9(4) .
O8D P8B O8 P8A 159.8(3) .
O8E P8B O8 P8A 39.0(4) .
O8F P8B O8 P8A -81.8(4) .
O9A P9A O9 P9B 129.9(4) .
O9B P9A O9 P9B -112.9(5) .
O9C P9A O9 P9B 8.0(5) .
O9D P9B O9 P9A -165.2(4) .
O9E P9B O9 P9A 76.6(5) .
O9F P9B O9 P9A -45.4(5) .
O10A P10A O10 P10B 133.7(4) .
O10B P10A O10 P10B -106.8(5) .
O10C P10A O10 P10B 13.3(5) .
O10D P10B O10 P10A -61.2(5) .
O10E P10B O10 P10A 60.5(5) .
O10F P10B O10 P10A 180.0(4) .
O11A P11A O11 P11B 90.1(4) .
O11B P11A O11 P11B -151.5(3) .
O11C P11A O11 P11B -30.6(4) .
O11D P11B O11 P11A -161.7(3) .
O11E P11B O11 P11A 78.7(4) .
O11F P11B O11 P11A -42.1(4) .
O12A P12A O12 P12B 71.5(4) .
O12B P12A O12 P12B -169.3(4) .
O12C P12A O12 P12B -49.8(5) .
O12D P12B O12 P12A -129.4(4) .
O12E P12B O12 P12A 113.3(4) .
O12F P12B O12 P12A -8.4(5) .
O13A P13A O13 P13B 154.0(6) .
O13B P13A O13 P13B -86.8(7) .
O13C P13A O13 P13B 33.6(7) .
O13D P13B O13 P13A -94.8(7) .
O13E P13B O13 P13A 26.5(7) .
O13F P13B O13 P13A 145.9(6) .
O14A P14 O14 P14 126.7(14) 5_666
O14B P14 O14 P14 4.8(17) 5_666
O14C P14 O14 P14 -118.9(14) 5_666
